advertisement

MECHANICAL PROPERTIES OF MATERIALS • • • • • Stress-Strain Relationships Hardness Effect of Temperature on Properties Fluid Properties Viscoelastic Behavior of Polymers ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 1 Mechanical Properties in Design and Manufacturing • Mechanical properties determine a material’s behavior when subjected to mechanical stresses Properties include elastic modulus, ductility, hardness, and various measures of strength • Dilemma: mechanical properties desirable to the designer, such as high strength, usually make manufacturing more difficult The manufacturing engineer should appreciate the design viewpoint and the designer should be aware of the manufacturing viewpoint ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 2 Stress-Strain Relationships • • Three types of static stresses to which materials can be subjected: 1. Tensile - tend to stretch the material 2. Compressive - tend to squeeze it 3. Shear - tend to cause adjacent portions of material to slide against each other Stress-strain curve - basic relationship that describes mechanical properties for all three types ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 3 Tensile Test • Most common test for studying stress-strain relationship, especially metals • In the test, a force pulls the material, elongating it and reducing its diameter Figure 3.1 - Tensile test: (a) tensile force applied in (1) and (2) resulting elongation of material ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 4 ASTM (American Society for Testing and Materials) specifies preparation of test specimen Figure 3.1 - Tensile test: (b) typical test specimen ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 5 Figure 3.1 - Tensile test: (c) setup of the tensile test ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 6 Figure 3.2 - Typical progress of a tensile test: (1) beginning of test, no load; (2) uniform elongation and reduction of cross-sectional area; (3) continued elongation, maximum load reached; (4) necking begins, load begins to decrease; and (5) fracture. If pieces are put back together as in (6), final length can be measured ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 7 Engineering Stress Defined as force divided by original area: F e Ao where e = engineering stress, F = applied force, and Ao = original area of test specimen ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 8 Engineering Strain Defined at any point in the test as L Lo e Lo where e = engineering strain; L = length at any point during elongation; and Lo = original gage length ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 9 Figure 3.3 - Typical engineering stress-strain plot in a tensile test of a metal ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 10 Two Regions of Stress-Strain Curve • The two regions indicate two distinct forms of behavior: 1. Elastic region – prior to yielding of the material 2. Plastic region – after yielding of the material ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 11 Elastic Region in Stress-Strain Curve • Relationship between stress and strain is linear • Material returns to its original length when stress is removed Hooke's Law: e = E e where E = modulus of elasticity • E is a measure of the inherent stiffness of a material • Its value differs for different materials ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 12 Yield Point in Stress-Strain Curve • As stress increases, a point in the linear relationship is finally reached when the material begins to yield Yield point Y can be identified by the change in slope at the upper end of the linear region Y = a strength property Other names for yield point = yield strength, yield stress, and elastic limit ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 13 Plastic Region in Stress-Strain Curve • Yield point marks the beginning of plastic deformation • The stress-strain relationship is no longer guided by Hooke's Law • As load is increased beyond Y, elongation proceeds at a much faster rate than before, causing the slope of the curve to change dramatically ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 14 Tensile Strength in Stress-Strain Curve • Elongation is accompanied by a uniform reduction in cross-sectional area, consistent with maintaining constant volume • Finally, the applied load F reaches a maximum value, and engineering stress at this point is called the tensile strength TS or ultimate tensile strength Fmax TS = Ao ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 15 Ductility in Tensile Test Ability of a material to plastically strain without fracture Lf Lo EL Lo where EL = elongation; Lf = specimen length at fracture; and Lo = original specimen length Lf is measured as the distance between gage marks after two pieces of specimen are put back together ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 16 True Stress Stress value obtained by dividing the instantaneous area into applied load F A where = true stress; F = force; and A = actual (instantaneous) area resisting the load ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 17 True Strain Provides a more realistic assessment of "instantaneous" elongation per unit length L dL L ln Lo L L o ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 18 If previous engineering stress-strain curve were plotted using true stress and strain values Figure 3.4 - True stress-strain curve for the previous engineering stress-strain plot in Figure 3.3 ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 19 Strain Hardening in Stress-Strain Curve • Note that true stress increases continuously in the plastic region until necking In the engineering stress-strain curve, the significance of this was lost because stress was based on an incorrect area value • What it means is that the metal is becoming stronger as strain increases This is the property called strain hardening ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 20 When the plastic region of the true stress-strain curve is plotted on a log-log scale, it becomes linear Figure 3.5 - True stress-strain curve plotted on log-log scale ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 21 Flow Curve Because it is a straight line in a log-log plot, the relationship between true stress and true strain in the plastic region is K n where K = strength coefficient; and n = strain hardening exponent ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 22 Categories of Stress-Strain Relationship 1. Perfectly elastic 2. Elastic and perfectly plastic 3. Elastic and strain hardening ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 23 Perfectly Elastic Behavior is defined completely by modulus of elasticity E • It fractures rather than yielding to plastic flow • Brittle materials: ceramics, many cast irons, and thermosetting polymers Figure 3.6 - Three categories of stress-strain relationship: (a) perfectly elastic ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 24 Elastic and Perfectly Plastic • Stiffness defined by E • Once Y reached, deforms plastically at same stress level • Flow curve: K = Y, n = 0 • Metals behave like this when heated to sufficiently high temperatures (above recrystallization) Figure 3.6 - Three categories of stress-strain relationship: (b) elastic and perfectly plastic ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 25 Elastic and Strain Hardening • Hooke's Law in elastic region, yields at Y • Flow curve: K > Y, n > 0 • Most ductile metals behave this way when cold worked Figure 3.6 - Three categories of stress-strain relationship: (c) elastic and strain hardening ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 26 Compression Test • Applies a load that squeezes the ends of a cylindrical specimen between two platens Figure 3.7 - Compression test: (a) compression force applied to test piece in (1) and (2) resulting change in height ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 27 Figure 3.7 - Compression test: (b) setup for the test with size of test specimen exaggerated ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 28 Engineering Stress in Compression As the specimen is compressed, its height is reduced and cross-sectional area is increased F e Ao where Ao = original area of the specimen ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 29 Engineering Strain in Compression Engineering strain is defined h ho e ho Since height is reduced during compression, value of e is negative (the negative sign is usually ignored when expressing compression strain) ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 30 • Shape of plastic region is different from tensile test because cross-section increases • Calculated value of engineering stress is higher Figure 3.8 - Typical engineering stress-strain curve for a compression test ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 31 Tensile Test vs. Compression Test • Although differences exist between engineering stress-strain curves in tension and compression, the true stress-strain relationships are nearly identical • Since tensile test results are more common, flow curve values (K and n) from tensile test data can be applied to compression operations • When using tensile K and n data for compression, ignore necking, which is a phenomenon peculiar to straining induced by tensile stresses ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 32 Testing of Brittle Materials • Hard brittle materials (e.g., ceramics) possess elasticity but little or no plasticity • Often tested by a bending test (also called flexure test) Specimen of rectangular cross-section is positioned between two supports, and a load is applied at its center ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 33 Figure 3.10 - Bending of a rectangular cross-section results in both tensile and compressive stresses in the material: (1) initial loading; (2) highly stressed and strained specimen; and (3) bent part ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 34 Testing of Brittle Materials • Brittle materials do not flex • They deform elastically until fracture Failure occurs because tensile strength of outer fibers of specimen are exceeded Failure type: cleavage - common with ceramics and metals at low temperatures, in which separation rather than slip occurs along certain crystallographic planes ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 35 Transverse Rupture Strength The strength value derived from the bending test: TRS 1.5FL bt 2 where TRS = transverse rupture strength; F = applied load at fracture; L = length of specimen between supports; and b and t are dimensions of cross-section ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 36 Shear Properties Application of stresses in opposite directions on either side of a thin element Figure 3.11 - Shear (a) stress and (b) strain ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 37 Shear Stress and Strain Shear stress defined as F A where F = applied force; and A = area over which deflection occurs. Shear strain defined as b where = deflection element; and b = distance over which deflection occurs ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 38 Figure 3.13 - Typical shear stress-strain curve from a torsion test ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 39 Shear Elastic Stress-Strain Relationship In the elastic region, the relationship is defined as G where G = shear modulus, or shear modulus of elasticity • For most materials, G 0.4E, where E = elastic modulus ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 40 Shear Plastic Stress-Strain Relationship • Relationship similar to flow curve • Shear stress at fracture = shear strength S Shear strength can be estimated from tensile strength: S 0.7(TS) • Since cross-sectional area of test specimen in torsion test does not change as in tensile and compression, engineering stress-strain curve for shear true stress-strain curve ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 41 Hardness Resistance to permanent indentation • Good hardness generally means material is resistant to scratching and wear • Most tooling used in manufacturing must be hard for scratch and wear resistance ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 42 Hardness Tests • Commonly used for assessing material properties because they are quick and convenient • Variety of testing methods are appropriate due to differences in hardness among different materials • Most well-known hardness tests are Brinell and Rockwell • Other test methods are also available, such as Vickers, Knoop, Scleroscope, and durometer ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 43 Brinell Hardness Widely used for testing metals and nonmetals of low to medium hardness • A hard ball is pressed into specimen surface with a load of 500, 1500, or 3000 kg Figure 3.14 - Hardness testing methods: (a) Brinell ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 44 Brinell Hardness Number Load divided into indentation area = Brinell Hardness Number (BHN) HB 2F Db (Db Db2 Di2 ) where HB = Brinell Hardness Number (BHN), F = indentation load, kg; Db = diameter of ball, mm, and Di = diameter of indentation, mm ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 45 Rockwell Hardness Test • Another widely used test • A cone shaped indenter is pressed into specimen using a minor load of 10 kg, thus seating indenter in material • Then, a major load of 150 kg is applied, causing indenter to penetrate beyond its initial position • Additional penetration distance d is converted into a Rockwell hardness reading by the testing machine ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 46 Figure 3.14 - Hardness testing methods: (b) Rockwell: (1) initial minor load and (2) major load ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 47 Effect of Temperature on Properties Figure 3.15 - General effect of temperature on strength and ductility ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 48 Hot Hardness Ability of a material to retain hardness at elevated temperatures Figure 3.16 - Hot hardness - typical hardness as a function of temperature for several materials ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 49 Recrystallization in Metals • Most metals strain harden at room temperature according to the flow curve (n > 0) • But if heated to sufficiently high temperature and deformed, strain hardening does not occur Instead, new grains are formed that are free of strain The metal behaves as a perfectly plastic material; that is, n = 0 ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 50 Recrystallization Temperature • Formation of new strain-free grains is called recrystallization • Recrystallization temperature of a given metal = about one-half its melting point (0.5 Tm) as measured on an absolute temperature scale • Recrystallization takes time - the recrystallization temperature is specified as the temperature at which new grains are formed in about one hour ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 51 Recrystallization and Manufacturing • Recrystallization can be exploited in manufacturing • Heating a metal to its recrystallization temperature prior to deformation allows a greater amount of straining, and lower forces and power are required to perform the process • Forming metals at temperatures above recrystallization temperature is called hot working ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 52 Fluid Properties and Manufacturing • Fluids flow • They take the shape of the container that holds them • Many manufacturing processes are accomplished on materials converted from solid to liquid by heating • Examples: Metals are cast in molten state Glass is formed in a heated and highly fluid state Polymers are almost always shaped as thick fluids ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 53 Viscosity in Fluids • Flow is a defining characteristic of fluids, but the tendency to flow varies for different fluids • Viscosity is the resistance to flow that is characteristic of a given fluid • Viscosity is a measure of the internal friction when velocity gradients are present in the fluid The more viscous the fluid, the higher the internal friction and the greater the resistance to flow Reciprocal of viscosity is fluidity - the ease with which a fluid flows ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 54 • Viscosity can be defined using two parallel plates separated by a distance d • A fluid fills the space between the two plates. Figure 3.17 - Fluid flow between two parallel plates, one stationary and the other moving at velocity v ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 55 Shear Stress Shear stress is the frictional force exerted by the fluid per unit area • Motion of the upper plate is resisted by a frictional force resulting from the shear viscosity of the fluid This force F can be reduced to a shear stress by dividing by plate area A F A ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 56 Shear Rate Shear stress is related to shear rate, which is defined as the change in velocity dv relative to dy dv dy where = shear rate, 1/s; dv = change in velocity, m/s; and dy = change in distance y, m • Shear rate = velocity gradient perpendicular to flow direction ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 57 Shear Viscosity Shear viscosity is the fluid property that defines the relationship between F/A and dv/dy; that is, F dv A dy or where = a constant of proportionality called the coefficient of viscosity, Pa-s • For Newtonian fluids, viscosity is a constant • For non-Newtonian fluids, it is not ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 58 Coefficient of Viscosity Rearranging, coefficient of viscosity can be expressed: Viscosity of a fluid is the ratio of shear stress to shear rate during flow ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 59 Viscosity of Polymers and Flow Rate • Viscosity of a thermoplastic polymer melt is not constant It is affected by flow rate Its behavior is non-Newtonian • A fluid that exhibits this decreasing viscosity with increasing shear rate is called pseudoplastic • This complicates analysis of polymer shaping processes such as injection molding ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 60 Figure 3.18 - Viscous behaviors of Newtonian and pseudoplastic fluids. Polymer melts exhibit pseudoplastic behavior. For comparison, the behavior of a plastic solid material is shown. ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 61 Viscoelastic Behavior Material property that determines the strain it experiences when subjected to combinations of stress and temperature over time • Combination of viscosity and elasticity ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 62 Figure 3.19 - Comparison of elastic and viscoelastic properties: (a) perfectly elastic response of material to stress applied over time; and (b) response of a viscoelastic material under same conditions. The material in (b) takes a strain that is a function of time and temperature. ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 63 Viscoelastic Behavior of Polymers: Shape Memory • A common problem in extrusion of polymers is die swell, in which the profile of extruded material grows in size, reflecting its tendency to return to its previously larger cross-section in the extruder barrel immediately before being squeezed through the smaller die opening It “remembers” ©2002 John Wiley & Sons, Inc. M. P. Groover, “Fundamentals of Modern Manufacturing 2/e” 64